|Year : 2019 | Volume
| Issue : 6 | Page : 112-125
Monomer modifications of denture base acrylic resin: A systematic review and meta-analysis
R Ajay1, K Suma2, Seyed Asharaf Ali2
1 Department of Prosthodontics and Crown and Bridge, Vivekanandha Dental College for Women, Tiruchengode, Tamil Nadu, India
2 Department of Prosthodontics and Crown and Bridge, Rajah Muthiah Dental College and Hospital, Annamalai University, Chidambaram, Tamil Nadu, India
|Date of Web Publication||28-May-2019|
Dr. R Ajay
Department of Prosthodontics and Crown and Bridge, Vivekanandha Dental College for Women, Elayampalayam, Tiruchengode, Namakkal 637205, Tamil Nadu
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Background: Methyl methacrylate monomer of denture base resins was modified with several monomers to achieve better physico-mechanical properties without compromising the biocompatibility. However, there are no consensuses on the best strategy to achieve best modified monomer. Purpose: To identify and evaluate the differences in the properties between conventional and modified monomers and to verify the influence of several variables on the properties of denture base acrylic resin. Materials and Methods: This study was executed by following the Preferred Reporting Items for Systematic Reviews and Meta-Analyses statement. In-vitro studies that investigated the properties of conventional and modified monomers were selected. Searches were carried out in the Ebscohost, PubMed, Semantic scholar and J-stage databases. The search commenced from the year 1995 and the last search was done till November 2018. A comparison was performed between modified and unmodified monomers. The analyses were carried out using fixed-effect models. Results: The meta-analysis results showed high heterogeneity in all aspects, and higher flexural strength for monomers modified with 20% methacrylic acid. Conclusion: Although the articles included in this meta-analysis showed high heterogeneity and high risk of bias, the in-vitro literature seems to suggest that use of modified monomers could improve the properties of denture base resins. Other variants of monomer modifications and their tested parameters were discussed in this systematic review as well. Dimensional accuracy is an unexplored variable to be evaluated extensively in the future researches.
Keywords: Monomer, Methyl-methacrylate, properties, biocompatibility
|How to cite this article:|
Ajay R, Suma K, Ali SA. Monomer modifications of denture base acrylic resin: A systematic review and meta-analysis. J Pharm Bioall Sci 2019;11, Suppl S2:112-25
|How to cite this URL:|
Ajay R, Suma K, Ali SA. Monomer modifications of denture base acrylic resin: A systematic review and meta-analysis. J Pharm Bioall Sci [serial online] 2019 [cited 2022 May 28];11, Suppl S2:112-25. Available from: https://www.jpbsonline.org/text.asp?2019/11/6/112/258866
| Introduction|| |
The field of prosthetic dentistry is null without dental materials. Both are inextricably connected to each other since they have evolved. Prosthodontists are the ones who encounter with multitudinous materials. A good dentist can aptly identify and use any given material whereas a good prosthodontist is an authoritative chemist who has engulfed the science of reactions and manipulations of the materials. An eternal friendship between a prosthodontist and denture base acrylic resins exists.
Poly(methyl methacrylate) (PMMA) is the most commonly used denture base material for the past 60 years. Although numerous denture base polymers have been invented and introduced into dentistry to overcome issues related with PMMA resin, it has remained the material of choice for the fabrication of denture bases. It is the combination of various desirable properties of PMMA resin that accounts for the universal consumption though its properties are not ideal in every aspect.
The limitations of heat-cured PMMA resin with respect to strength, peculiarly under impact and fatigue conditions, were investigated by several researchers. The use of alternative materials with considerable improvement in strength would resist the denture fracture though it might be minimized by proper denture design and by following appropriate fabrication techniques.,
Also, the prosthesis installation within the oral cavity changes the bio-environment and paves the way for the deposition of biofilms on the prosthetic device. The porous and irregular surfaces of acrylic resins favor microbial adhesion, accumulation, and colonization, which are determining agents in the majority of oral problems such as candidiasis, sore/burning mouth, and glossodynia., PMMA resin with antimicrobial properties would be ideal to improve the patients’ quality of life and to impede discomfort with cost-effectiveness. Handful of studies have aimed at reducing or eliminating bacterial and fungal contamination by addition of antimicrobial agents, without compromising or rather deteriorating the mechanical properties of dental materials.
In the recent years, several modifications have been experimented in the denture base PMMA resins to improvise the physico-mechanical and biological properties. These modifications can be broadly classified into polymer and monomer modifications. The advances in polymer technology have produced novel polymers such as high-impact polymers and fiber-reinforced polymers with improved impact strength and fatigue resistance. The polymer modifications are achieved either by incorporating additives such as rubber, styrene-butadiene, Al2O3, and β-AgVO3 or by adding inorganic fillers such as metallic oxides, fluorinated glass fillers, hydroxyapatite whiskers, zirconia, and organic fibers of carbon/graphite, aramid, ultra-high modulus polyethylene, nylon, and jute. Reviews of studies regarding the polymeric modifications are available in the dental literature.,,, However, literature reviews on monomer modifications are not available yet.
The purpose of this study was to (1) systematically review the published researches pertaining to the modifications of denture base acrylic resin monomer, and (2) identify tests used for physico-mechanical and biological properties analysis.
| Materials andMethods|| |
Patient intervention comparison outcome model includes studies pertaining to denture base acrylic resins. Intervention was the quantitative modification of the monomer. Comparators were the conventional monomers without modifications. Outcomes were the effect of modified monomers on the properties of denture base acrylic resins.
The electronic search was independently performed by two reviewers. The databases used for search were EBSCOhost (http://web.a.ebscohost.com/ehost/publication), PubMed (www.ncbi.nlm. nih.gov. /entrez/ query.fcgi), Semantic Scholar (https://www.semanticscholar.org/search), and J-STAGE (https://www.jstage.jst.go.jp). The present systematic review included research titles published from the year 1995 to 2018 in which comparison between unmodified and modified monomers was executed. On the basis of MeSH terms (PubMed), Boolean phrases (EBSCOhost), and other free-term keywords such as denture bases, monomers, polymethyl methacrylate, methacrylates, methylmethacrylate, methacrylic acid, denture base resins, denture base monomers, denture base modified monomers, modified denture bases, denture base co-monomer, monomer modification, anti-microbial monomer, anti-fungal monomer, denture base novel monomer, and denture base properties, the studies were assessed for the relevance. In case of any disagreement regarding the inclusion of a study, a third reviewer was consulted to achieve a consensus. Full texts of all relevant research studies that satisfied the inclusion criteria were downloaded. No blinding was carried out regarding the authors, journals, date of publication, or results.
Inclusion and exclusion criteria
Three main aspects were considered when reports were identified for inclusion: substratum, material, and testing methods. Eligible substrata consisted of modifications made in the monomer as liquid substitute and volume percentage of the monomer substitute. The exclusion criteria included studies pertaining to the monomers of light-cure composite resins, monomers of dental adhesives, pits and fissure sealants, and monomers of tissue conditioners and soft lining materials.
A data extraction criterion was defined and assessed by two authors. The data were extracted from the full-text articles selected independently. The authors classified the information on authors/year, monomer, its availability, monomer added to proprietary monomer (MMA) in percent, denture base materials, polymer/monomer (P/L) ratio, curing regimen, property studied, results, conclusions, and risk of bias.
Assessment of risk of bias
Risk of bias was evaluated according to the articles’ elucidation of the following parameters: randomization of samples/specimens, use of control group, use of materials according to the manufacturer’s instructions, preparation of samples according to ISO/ADA/ANSI standards with dimensions, sample preparation by the single operator, description of sample-size calculation, and blinding of the operator of the testing machine. Articles with one-to-three reported items were classified to possess high risk of bias, four or five reported items as medium risk of bias, and six or seven reported items as low risk of bias.,,
Considering the heterogeneity of the studies with respect to research design, methodology executed, sample sizes, storage, and polymerization method, only studies that met particular criteria were included in the meta-analysis. For flexural strength, the inclusion criteria were the following: moderate or high risk of bias; compliance with ISO standards for specimen dimension, and P/L ratio; reported means and standard deviations for the groups. The wt/vol% of substituted monomer (MAA) into the proprietary monomer (MMA) was kept constant (20%) to avoid heterogeneity. When the studies were similar in terms of these substrata, heterogeneity was further evaluated through the Q, I2, and τ2 tests.
The fixed-effect and random-effects models were considered appropriate for the meta-analysis of any quantitative data. However, considering the substrata, fixed-effect model was executed. In this review, it was possible to group four studies that evaluated the modified monomer (MAA). Other forms of evaluations such as publication bias and subgroup analysis were precluded because of insufficient number of included studies. All analyses were executed with statistical software (Comprehensive Meta-Analysis; version 3, Biostatistics).
| Results|| |
Search and selection
A total of 308 titles were obtained through the electronic search. Once duplicates, studies not relevant to the research question, and articles not in English were excluded; only 54 full-text articles were left. Thirty-four studies where the methodology for modification was not elucidated and monomer modifications were performed by incorporation of inorganic nanoparticle powder in monomer were further excluded. Finally, 20 studies were considered suitable for the present systematic review [Figure 1]. The exclusion criteria according to CONSORT* included incomplete description of materials, methods or details of the experimental procedure, not following standardized testing protocols, absence of sample size calculation, incomplete or inappropriate statistical analysis, no conflict of interests statement, limited interpretation, and comparison of results with other available dental literature.
Risk of bias
From the 28 researches evaluating the properties of denture base acrylic resin with modified monomers, 17 researches presented a moderate risk of bias and only 11 presented high risk of bias. The most common risks of bias in the studies evaluating modified monomers were the sample randomization, sample preparation by a single operator, calculation for sample size, and blinding the operator of the testing machine. The studies evaluating modified monomers scored exclusively poor with respect to the sample randomization, sample preparation by a single operator, sample size calculations, and blinding protocols.
The 80% MMA + 20% MAA group showed significantly higher flexural strength than the 100% MMA group [Figure 2]. The heterogeneity of the four studies included in the meta-analysis was high (Q = 68.525, heterogeneity P = 0.000, I2 = 95.62%, τ2 = 6.051).
From the included researches in the systematic review, the modification of MMA was done basically by certain monomers or solutions that can be categorized as fluoromonomers,,,, (n = 5), phosphate monomers,, (n = 3), methacrylic acid monomer,,,,, (n = 6), itaconate monomers,, (n = 3), nitromonomers,,,, (n = 5), and nonspecific monomers or solutions (n = 6). Nonspecific monomers include Norbonyl/phenyl methacrylate (NBMA/PHMA), polyhedral oligosilsesquioxane (POSS), methacrylated dendrimer (DD1), 1,3-bis(3-methacryloxypropyl)-1, 1, 3, 3 tetramethyl disiloxane (BMPMS), silver nitrate (AgNO3) solution, and N-acetyl cysteine (NAC).
The monomers used to substitute with MMA (wt/vol%) were either experimentally synthesized,,,,,, or purchased.,,,,,,,,,,,,,,,,,,, For the specimen preparation, the polymer beads were synthesized by bulk polymerization,,,, suspension polymerization,,,,, or from the commercially available pre-polymers. The commercially available pre-polymers used were Lucitone 550,,,, Lucitone 199,, Paladent 20, Trevalon, Vertex,, DPI,, Ondacryl, Ivoclar Vivadent, Biocryl,,, QC-20, Acron MC, and Uniffasttrad. Researches included in this review, based upon the polymerization process, used heat-cured PMMA resin,[29-32],,,,,,,,,,,,,,,, autopolymerizing resin,,,,,,, and microwave irradiation.,
From [Table 1], it can be understood that a number of curing regimens were followed and executed for both heat-cured and microwave-irradiated specimen preparations. The activator used in autopolymerizing resin were AIBN,,,N,N-dimethyl-p-toluidine, and N,N-dimethyl aniline. The substitution of the monomers to MMA in wt/vol% is critical. For perfluoroalkylethyl acrylate monomers, polymer beads were not formed beyond 25 wt%.,, Also, the wt/vol% of substituted monomer affects the dough-forming time, which was recorded and mentioned in two, of the selected researches. In all the studies, the control group (0%) was used to compare with the monomer-substituted groups. A vivid wt/vol% of substituted monomers into the proprietary monomer was demonstrated. The most commonly executed wt/vol% of substituted monomer were 10%,,,,,,,,,,,,,,, and 20%.,,,,,,,,,,,
Vivid description about the testing methodologies of the properties in each of the studies was provided. All the aspects of the properties of the denture base resins were studied. However, the polymerization shrinkage, which is the commonest troubleshoot, has been studied only in one study. Every single study included here followed the standardized testing protocols, inclusive of specimen dimensions, stipulated for denture base resins.
| Discussion|| |
Fluoromonomers have an inherent property of “water-shedding” because of the fluorine ions; thus they possess hydrophobicity and have been exploited in the field of prosthetic dentistry. This is a novel approach by substituting fluoromonomers in MMA and reducing the water sorption, less acute contact angle,, and thus decreased microbial adhesion especially Candidal adhesion as far as denture stomatitis is concerned., These monomers were also incorporated in the proprietary monomers of denture soft/resilient liners, to reduce the water sorption and solubility in oral environment and to curb the Candidal adhesion. Nevertheless, the effect of fluoromonomers on glass transition temperature, (Tg), surface hardness,, surface roughness (Ra), tensile,, compressive, and flexural strength, were also investigated. Though this addition causes some deterioration to the mechanical properties, it can be acceptable for clinical use. Extensive biocompatibility assay has to be executed with this monomer.
Addition of phosphate monomers to MMA caused increased water sorption, solubility, and more acute contact angles. From these results, it is inferred that these monomers are hydrophilic in nature. Performance of these monomers with respect to color stability and staining was acceptable. Though there is slight decrease in the mechanical properties such as flexural strength, impact strength, and fracture toughness, there were no devastating effects stating its limitations in clinical usage. However, it is also said to be an antifungal monomer by inhibiting the adhesion and colonization of Candida albicans. Moreover, there is a huge lacuna with respect to the biocompatibility assays for these groups of monomers.
Methacrylic acid (MAA) is primarily an antimicrobial monomer substituted in MMA. MAA decreased the microbial adhesion, and also had more acute contact angle. The hydrophilicity of this monomer has to be extensively studied with respect to water sorption and solubility. Substitution of MAA improved the surface roughness., Chemical characterization and copolymerization was demonstrated when added to MMA. MAA caused reduction in surface hardness. With respect to flexural strength, antonymous conclusions were demonstrated stating both increased, and decreased, flexural strength (FS) upon MAA substitution. This monomer is also open for the future impact strength and biocompatibility tests.
Evidence of copolymerization was demonstrated when itaconate monomers were added to MMA. Residual monomer content was significantly reduced with the substitution of itaconate monomers in MMA. This is due to the increase in degree of conversion of the monomers to polymeric units., Water sorption increased with increasing concentrations of itaconate monomers., Glass transition temperature and tensile strength decreased with itaconates. Dimethyl itaconate compromised the impact strength and di-tetrahydro furfuryl itaconate reduced the surface hardness. Light has to be thrown with respect to flexural strength and biocompatibility assays with these monomers.
Nitromonomer is a new term introduced here for the convenience of explanation about some nitrogen-containing monomers in the form of either amino/ammonium/pyridinium or amides. These monomers can be also tagged as antimicrobial monomers. High N2 ratio and copolymerization were demonstrated when 2-tert-butyl aminoethyl methacrylate (TBAEMA) was added to MMA. Reduced flexural strength, Tg, and increased water sorption at raised concentrations were also observed., Quaternized ammonium monomer (DMAEMA-OB) was effective against gram-positive and gram-negative bacteria and fungi. Another quaternized ammonium anti-microbial monomer (QAM), 2-(methacryloyloxy) ethyl trimethyl ammonium chloride (MADQUAT), was proved to be an efficient antifungal monomer possessing both fungistatic and -cidal actions. However, its copolymerization with MMA, physico-mechanical properties, and biocompatibility are yet unknown.
Numerous novel QAMs were synthesized and were experimented with dental restorative composite and adhesive resins. Dimethylaminododecyl methacrylate (DMADDM) and dimethylammoniumethyl dimethacrylate (DMAEDM) were found to possess “time-kill” antibacterial properties. Both monomers had significantly lesser cytotoxicity than the bisphenol A-glycidyl methacrylate (Bis-GMA). DMADDM was proved to be an antimicrobial denture base monomer against the formation of multispecies biofilm on the denture surfaces. It changed the structure of multi-biofilm and inhibited the biofilm metabolic activities, hyphal development, and virulence-related genes’ expression of C. albicans. It also reduced the Candidal receptors on the host cells, thus reducing cell damage as well as being biocompatible at a concentration of 1.65–3.3%. Methacryloxyethyl cetyl dimethyl ammonium chloride (DMAE-CB) can be used as an antibacterial monomer by incorporating into dental restorative materials. Unpolymerized 2-methacryloxyethyl dodecyl methyl ammonium bromide (MAE-DB) and 2-methacryloxyethyl hexadecyl methyl ammonium bromide (MAE-HB) cross-linking monomers showed a strong bactericidal activity against eight different strains of oral bacteria. They had significantly lesser cytotoxicity than that of Bis-GMA. These monomers have a unique property of “contact-kill.” Any microorganism that comes in contact with the denture base containing QAM gets killed. QAM intrinsically possessing positive charge has high affinity toward negatively charged cell membrane; it disrupts the lipid bilayer, leads to leakage of intracellular accessories, and eventually results in microbial death. They can be also designated as cationic monomers. These QAMs, however, have a wide scope of research in developing newer denture base resins.
Two pyridinium-based nitromonomers were used in dentistry. Methacryloyl oxyundecyl pyridinium bromide (MUPB) added to MMA reduced the flexural strength, whereas surface roughness, hardness, and color stability were unaffected. Methacryloyloxy-dodecyl-pyridinium-bromide (MDPB) is being extensively used in the field of research pertained to restorative resins as bactericidal monomer against oral bacteria. The cytotoxicity was similar to those of other monomers used in dental materials. Acrylamide monomer in MMA increased the flexural strength and modulus by copolymerizing with PMMA.
NBMA and PHMA are hydrophobic monomers that reduced water sorption and improved the mechanical properties. NBMA with MMA showed less polymerization shrinkage, and this may be attributed to the fact that norbonyl compounds polymerize through ring-opening metathesis polymerization (ROMP). POSS with MMA at all experimental concentrations yielded lesser cytotoxicity than the PMMA. DD1 with MMA did not affect the flexural strength and surface hardness. Water sorption and solubility decreased significantly with the addition of BMPMS with MMA, and thus, can be considered as hydrophobic monomer. Substituting AgNO3 solution with MMA increased impact strength at 60ppm concentration. Discoloration was observed at 300ppm. This is because of the oxidative reaction of Ag with the atmosphere. With increase in the concentration, the flexural and tensile strength decreased. NAC is a cellular friendly product, and hence, showed higher cell viability when added to MMA. Surface roughness and hardness were affected at a concentration beyond 0.3% and 0.15%, respectively. Flexural strength decreased with increasing concentrations of NAC.
In this systematic review, the selected studies evaluated only the experimental monomers and commercially available products using these monomers are yet to be launched in the market.
| Limitations|| |
Cautious interpretations of the results of the present review are mandatory because in vitro laboratory experiments have intrinsic limitations while trying to simulate oral conditions such as masticatory loads, masticatory cycles, temperature fluctuations, microbial flora, and salivary flow rate. Properly designed randomized controlled trials with long follow-up duration are essential to deduce at a conclusion as to whether monomer modifications will result in improved clinical success rates when compared with conventional PMMAs. None of the studies included have a complete research about a monomer, especially with respect to dimensional accuracy of denture base.
| Conclusion|| |
- Monomer modification improved the physico-mechanical properties and biocompatibility of the denture base resins.
- Though some monomers compromised specific properties, their performance in the clinical scenario is well accepted.
- Evaluation of dimensional stability/accuracy should be given high priority because it leads to several problems such as pain, tissue irritation, hyperplastic tissues, and occlusal errors.
- Numerous explicit researches to be undertaken to develop an ideal denture base resin because commercially available products do not suffice the geriatric population.
- Numerous antimicrobial monomers used with restorative resins shall be experimented with denture base resins to reduce microbial adhesion.
- Combination of two or more monomers of different inherent properties may be attempted and patented for commercial manufacture.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
al-Mulla MA, Murphy WM, Huggett R, Brooks SC. Effect of water and artificial saliva on mechanical properties of some denture-base materials. Dent Mater 1989;5:399-402.
Anderson GC, Schulte JK, Arnold TG. Dimensional stability of injection and conventional processing of denture base acrylic resin. J Prosthet Dent 1988;60:394-8.
Anthony DH, Peyton FA. Evaluating dimensional accuracy of denture bases with a modified comparator. J Prosthet Dent 1959;9:683-92.
Anthony DH, Peyton FA. Dimensional accuracy of various denture-base materials. J Prosthet Dent 1962;12:67-81.
Rodriguez LS, Paleari AG, Giro G, de Oliveira Junior NM, Pero AC, Compagnoni MA. Chemical characterization and flexural strength of a denture base acrylic resin with monomer 2-tert
-butylaminoethyl methacrylate. J Prosthodont 2013;22:292-7.
Valentini F, Luz MS, Boscato N, Pereira-Cenci T. Biofilm formation on denture liners in a randomised controlled in situ trial. J Dent 2013;41:420-7.
Wady AF, Machado AL, Zucolotto V, Zamperini CA, Berni E, Vergani CE. Evaluation of Candida albicans
adhesion and biofilm formation on a denture base acrylic resin containing silver nanoparticles. J Appl Microbiol 2012;112:1163-72.
Fan C, Chu L, Rawls HR, Norling BK, Cardenas HL, Whang K. Development of an antimicrobial resin—A pilot study. Dent Mater 2011;27:322-8.
Gjorgievska E, Apostolska S, Dimkov A, Nicholson JW, Kaftandzieva A. Incorporation of antimicrobial agents can be used to enhance the antibacterial effect of endodontic sealers. Dent Mater 2013;29:e29-34.
Jagger DC, Harrison A, Jandt KD. The reinforcement of dentures. J Oral Rehabil 1999;26:185-94.
Rodford R. The development of high impact strength denture-base materials. J Dent 1986;14:214-7.
Yadav NS, Elkawash H. Flexural strength of denture base resin reinforced with aluminium oxide and processed by different processing techniques. J Adv Dent Res 2011;2:33-6
de Castro DT, Valente ML, Agnelli JA, Lovato da Silva CH, Watanabe E, Siqueira RL, et al
. In vitro study of the antibacterial properties and impact strength of dental acrylic resins modified with a nanomaterial. J Prosthet Dent 2016;115:238-46.
Nuñez-Anita RE, Acosta-Torres LS, Vilar-Pineda J, Martínez-Espinosa JC, de la Fuente-Hernández J, Castaño VM. Toxicology of antimicrobial nanoparticles for prosthetic devices. Int J Nanomedicine 2014;9:3999-4006.
Al-Bakri IA, Harty D, Al-Omari WM, Swain MV, Chrzanowski W, Ellakwa A. Surface characteristics and microbial adherence ability of modified polymethylmethacrylate by fluoridated glass fillers. Aust Dent J 2014;59:482-9.
Pan Y, Liu F, Xu D, Jiang X, Yu H, Zhu M. Novel acrylic resin denture base with enhanced mechanical properties by incorporation of PMMA-modified hydroxyapatite. Mater Int 2013;23:89-93.
Ayad NM, Badawi MF, Fatah AA. Effect of reinforcement of high-impact acrylic resin with zirconia on some physical and mechanical properties. Rev Clín Pesq Odontol 2008;4:145-51.
Vallittu PK. A review of fiber-reinforced denture base resins. J Prosthodont 1996;5:270-6.
Alla RK, Sajjan S, Alluri VR, Ginjupalli K, Upadhya N. Influence of fiber reinforcement on the properties of denture base resins. J Biomater Nanobiotechnol 2013;4:91-7. doi: 10.4236/jbnb.2013.41012
Vallittu PK. A review of methods used to reinforce polymethyl methacrylate resin. J Prosthodont 1995;4:183-7.
Gad MM, Fouda SM, Al-Harbi FA, Näpänkangas R, Raustia A. PMMA denture base material enhancement: A review of fiber, filler, and nanofiller addition. Int J Nanomedicine 2017;12:3801-12.
Maia LC, Antonio AG. Systematic reviews in dental research: A guideline. J Clin Pediatr Dent 2012;37:117-24.
Astudillo-Rubio D, Delgado-Gaete A, Bellot-Arcís C, Montiel-Company JM, Pascual-Moscardó A, Almerich-Silla JM. Mechanical properties of provisional dental materials: A systematic review and meta-analysis. PLos One 2018;13:e0193162.
Sarkis-Onofre R, Skupien JA, Cenci MS, Moraes RR, Pereira-Cenci T. The role of resin cement on bond strength of glass-fiber posts luted into root canals: a systematic review and meta-analysis of in vitro studies. Oper Dent 2014;39:E31-44.
Moher D, Liberati A, Tetzlaff J, Altman DG; PRISMA Group. Preferred Reporting Items for Systematic Reviews and Meta-Analyses: The PRISMA statement. J Clin Epidemiol 2009;62:1006-12.
Hayashi R, Kubota T, Mega J. Application of fluoroalkyl acrylate monomer for a denture base material. Int J Oral-Med Sci 2003;1:124-9.
Kubota T, Kobayashi M, Hayashi R, Ono A, Mega J. Influence of carbon chain length of fluorinated alkyl acrylate on mechanical properties of denture base resin. Int J Oral-Med Sci 2005;4:92-6.
Kobayashi M, Kubota T, Mega J. Application of fluorinated alkyl acrylate to denture base resin. Influence of carbon chain length of fluorinated alkyl acrylate on bacterial adherence. Int J Oral-Med Sci 2006;4:136-41.
Kurata S, Morishita K, Shimoyama K, Umemoto K. Basic study on the application of novel functional monomers to a denture base resin. Dent Mater J 2008;27:273-7.
Cunha TR, Regis RR, Bonatti MR, de Souza RF. Influence of incorporation of fluoroalkyl methacrylates on roughness and flexural strength of a denture base acrylic resin. J Appl Oral Sci 2009;17:103-7.
Dhir G, Berzins DW, Dhuru VB, Periathamby AR, Dentino A. Physical properties of denture base resins potentially resistant to Candida
adhesion. J Prosthodont 2007;16:465-72.
Puri G, Berzins DW, Dhuru VB, Raj PA, Rambhia SK, Dhir G, et al
. Effect of phosphate group addition on the properties of denture base resins. J Prosthet Dent 2008;100:302-8.
Raj PA, Dentino AR. New phosphated poly(methyl methacrylate) polymers for the prevention of denture-induced microbial infection: An in vitro study. Clin Cosmet Investig Dent 2011;3:25-32.
Park SE, Periathamby AR, Loza JC. Effect of surface-charged poly(methyl methacrylate) on the adhesion of Candida albicans
. J Prosthodont 2003;12:249-54.
Azevedo AM, Regis RR, Chaves CAL, Souza RF, Fernandes RM. Physical properties of a denture base acrylic resins after incorporation of anionic charges. Rev Odontol Bras Central 2010;19:290-4.
Jain T, Yadav NS, Pandita A, Feroz SM, Kartika UK, Singh PP. A comparative evaluation of flexural strength of commercially available acrylic and modified polymethylmethacrylate: An in vitro study. J Contemp Dent Pract 2013;14:80-3.
Al-Ali AAS, Kassab-Bashi TY. Fourier transform infra red (FTIR) spectroscopy of new copolymers of acrylic resin denture base materials. Int J Enhanced Res Sci Tech Eng 2015;4:172-80.
Gupta L, Aparna IN, Bhat S, Ginjupalli K. Effect of comonomer of methacrylic acid on flexural strength and adhesion of Staphylococcus aureus
to heat polymerized poly (methyl methacrylate) resin: An in vitro
study. J Indian Prosthodont Soc 2017;17:149-55.
Sujitha K, Bharathi M, Lakshminarayana S, Shareef A, Lavanya B, SivKumar V. Physical properties of heat cure denture base resin after incorporation of methacrylic acid. Contemp Clin Dent 2018;9:251-5.
] [Full text]
Spasojević P, Stamenković D, Pjanović R, Bošković-Vragolović N, Dolić J, Grujić S, et al
. Diffusion and solubility of commercial poly(methyl methacrylate) denture base material modified with dimethyl itaconate and di-n
-butyl itaconate during water absorption/desorption cycles. Polym Int 2012;61. doi: 10.1002/pi.4202.
Spasojević P, Zrilić M, Panic V, Stamenkovic D, Seslija S, Velickovic S. The mechanical properties of a poly(methyl methacrylate) denture base material modified with dimethyl itaconate and di-n
-butyl itaconate. Int J Polym Sci 2015:1-9:doi: 10.1155/2015/561012.
Spasojević P, Panić V, Šešlija S, Nikolić V, Popović IG, Velicković S. Poly(methyl methacrylate) denture base materials modified with ditetrahydro furfuryl itaconate: Significant applicative properties. J Serb Chem Soc 2015;80:1177-92.
Paleari AG, Marra J, Pero AC, Rodriguez LS, Ruvolo-Filho A, Compagnoni MA. Effect of incorporation of 2-tert
-butylaminoethyl methacrylate on flexural strength of a denture base acrylic resin. J Appl Oral Sci 2011;19:195-9.
Mirizadeh A, Atai M, Ebrahimi S. Fabrication of denture base materials with antimicrobial properties. J Prosthet Dent 2018;119:292-8.
Regis RR, Zanini AP, Della Vecchia MP, Silva-Lovato CH, Oliveira Paranhos HF, de Souza RF. Physical properties of an acrylic resin after incorporation of an antimicrobial monomer. J Prosthodont 2011;20:372-9.
Aydogan Ayaz E, Durkan R. Influence of acrylamide monomer addition to the acrylic denture-base resins on mechanical and physical properties. Int J Oral Sci 2013;5:229-35.
Umemoto K, Kurata S. Basic study of a new denture base resin applying hydrophobic methacrylate monomer. Dent Mater J 1997;16:21-30.
Kim SK, Heo SJ, Koak JY, Lee JH, Lee YM, Chung DJ, et al
. A biocompatibility study of a reinforced acrylic-based hybrid denture composite resin with polyhedraloligosilsesquioxane. J Oral Rehabil 2007;34:389-95.
Kawaguchi T, Lassila LV, Vallittu PK, Takahashi Y. Mechanical properties of denture base resin cross-linked with methacrylated dendrimer. Dent Mater 2011;27:755-61.
Aoyagi Y, Umemoto K, Kurata S. Chemical properties of 1,3-bis(3-methacryloxypropyl)-1,1,3,3-tetramethyldisiloxane-methyl methacrylate copolymer. Dent Mater J 2012;31: 215-8.
Al-Husayni OKA, Hatoor NAF. Effect of silver nitrate incorporation into heat polymerized acrylic resin on some mechanical properties. J Bagh College Dentistry 2014;26:78-85.
Jiao Y, Ma S, Li J, Shan L, Yang Y, Li M, et al
. The influences of N
-acetyl cysteine (NAC) on the cytotoxicity and mechanical properties of poly-methylmethacrylate (PMMA)-based dental resin. PeerJj 2015;3:e868.
Hayakawa I, Akiba N, Keh E, Kasuga Y. Physical properties of a new denture lining material containing a fluoroalkyl methacrylate polymer. J Prosthet Dent 2006;96:53-8.
Yoshida K, Kurogi T, Torisu T, Watanabe I, Murata H. Effects of 2,2,2-trifluoroethyl methacrylate on properties of autopolymerized hard direct denture reline resins. Dent Mater J 2013;32:744-52.
Stopiglia CD, Collares FM, Ogliari FA, Piva E, Fortes CB, Samuel SM, et al
. Antimicrobial activity of [2-(methacryloyloxy)ethyl]trimethylammonium chloride against Candida
spp. Rev Iberoam Micol 2012;29:20-3.
Li F, Weir MD, Fouad AF, Xu HH. Time-kill behaviour against eight bacterial species and cytotoxicity of antibacterial monomers. J Dent 2013;41:881-91.
Zhang K, Ren B, Zhou X, Xu HH, Chen Y, Han Q, et al
. Effect of antimicrobial denture base resin on multi-species biofilm formation. Int J Mol Sci 2016;17:1033. doi:10.3390/ijms17071033.
Xiao YH, Chen JH, Fang M, Xing XD, Wang H, Wang YJ, et al
. Antibacterial effects of three experimental quaternary ammonium salt (QAS) monomers on bacteria associated with oral infections. J Oral Sci 2008;50:323-7.
Huang L, Xiao YH, Xing XD, Li F, Ma S, Qi LL, et al
. Antibacterial activity and cytotoxicity of two novel cross-linking antibacterial monomers on oral pathogens. Arch Oral Biol 2011;56:367-73.
Imazato S, Ebi N, Tarumi H, Russell RR, Kaneko T, Ebisu S. Bactericidal activity and cytotoxicity of antibacterial monomer MDPB. Biomaterials 1999;20:899-903.
[Figure 1], [Figure 2]
|This article has been cited by|
||Study on the Synthesis of Water-dispersible Acrylic Resin Containing Hydroxyl Group`
| ||Ma Jing, Mu Rong, Daowei Lai, Huaming Li, Yong Tao, Xiao Fei, Chunyu Zhou, Chufeng Sun, J. Xiao, X. Wu |
| ||MATEC Web of Conferences. 2022; 358: 01021 |
|[Pubmed] | [DOI]|
||Evaluation of Cytocompatibility of Thermopolymerized Denture Base Copolymer Containing a Novel Ring-opening Oxaspiro Comonomer
| ||Ranganthan Ajay, Ramajayam Sasikala, Vikraman Rakshagan, Jayaraman Raghunathan, Vellingiri LalithaManohari, Kandasamy Baburajan |
| ||World Journal of Dentistry. 2022; 13(2): 127 |
|[Pubmed] | [DOI]|
||Histocompatibility of Thermopolymerized Denture Base Copolymer Processed with a Novel Ring-opening Oxaspiro Comonomer: A Histomorphometric Investigation in Rats
| ||Ranganthan Ajay, Ramajayam Sasikala, Chandrasekaran Divagar, Boaz Ebenezer Solomon, Velayudhan Anand, Ghiaz Khalid |
| ||The Journal of Contemporary Dental Practice. 2022; 22(11): 1281 |
|[Pubmed] | [DOI]|
||Chemical Characterization and Physical Properties of Dental Restorative Composite Resin with a Novel Multifunctional Cross-linking Comonomer
| ||Ranganthan Ajay, Jambai Sampathkumar Sivakumar, Venkatesan Sudhakar, Chandramohan Ravivarman, Sundaravadivel Vignesh, Shafie Ahamed |
| ||The Journal of Contemporary Dental Practice. 2021; 22(6): 630 |
|[Pubmed] | [DOI]|
||Synthesis and characterization of a ring-opening oxaspiro comonomer by a novel catalytic method for denture base resins
| ||Ranganathan Ajay, Vikraman Rakshagan, Rajamani Ganeshkumar, Elumalai Ambedkar, Shafiullah RahmathShameem, Kanagesan Praveena |
| ||Journal of Pharmacy And Bioallied Sciences. 2021; 13(5): 521 |
|[Pubmed] | [DOI]|
||Copolymerization of ring-opening oxaspiro comonomer with denture base acrylic resin by free-radical/cationic hybrid polymerization
| ||Ranganathan Ajay, Vikraman Rakshagan, Murugesan Sreevarun, Dharanividhya Bhuvaneshkumar, Sekaran SajidaBegum, Veerakumar Vignesh |
| ||Journal of Pharmacy And Bioallied Sciences. 2021; 13(5): 527 |
|[Pubmed] | [DOI]|
||Quality assessment tools used in systematic reviews of in vitro studies: A systematic review
| ||Linh Tran, Dao Ngoc Hien Tam, Abdelrahman Elshafay, Thao Dang, Kenji Hirayama, Nguyen Tien Huy |
| ||BMC Medical Research Methodology. 2021; 21(1) |
|[Pubmed] | [DOI]|
||Evaluation of Porosity and Water Sorption in Conventionally Cured Modified Polymethyl Methacrylate Resin - An In Vitro Study
| ||Merin Mathew, Kamalakanth Shenoy, Ravishankar K. S. |
| ||Journal of Evolution of Medical and Dental Sciences. 2021; 10(13): 930 |
|[Pubmed] | [DOI]|
||Effect of novel cycloaliphatic comonomer on the flexural and impact strength of heat-cure denture base resin
| ||Ajay Ranganathan, Suma Karthigeyan, Rahila Chellapillai, Venkateshwaran Rajendran, Tamizhesai Balavadivel, Anand Velayudhan |
| ||Journal of Oral Science. 2021; 63(1): 14 |
|[Pubmed] | [DOI]|
||Histocompatibility of novel cycloaliphatic comonomer in heat-cured denture base acrylic resin: Histomorphometric analysis in rats
| ||Ranganathan Ajay, Karthigeyan Suma, Sengottaiyan Arulkumar, Ravichandran Mahadevan, Elumalai Ambedkar, KatturkaranAntonisamy Biju |
| ||Journal of Pharmacy And Bioallied Sciences. 2020; 12(5): 453 |
|[Pubmed] | [DOI]|
||Effect of novel cycloaliphatic comonomer on surface roughness and surface hardness of heat-cure denture base resin
| ||Ranganathan Ajay, Karthigeyan Suma, Vikraman Rakshagan, Elumalai Ambedkar, Vellingiri Lalithamanohari, Murugesan Sreevarun |
| ||Journal of Pharmacy And Bioallied Sciences. 2020; 12(5): 67 |
|[Pubmed] | [DOI]|
||Chemical Structure and Physical Properties of Heat-cured Poly(methyl methacrylate) Resin Processed with Cycloaliphatic Comonomer: An In Vitro Study
| ||Ranganthan Ajay, Karthigeyan Suma, Ramajayam Sasikala, Sekaran Sajidabegum, Veerakumar Vignesh, Dharanividhya Bhuvaneshkumar |
| ||The Journal of Contemporary Dental Practice. 2020; 21(3): 285 |
|[Pubmed] | [DOI]|
||Chemical Characterization of Denture Base Resin with a Novel Cycloaliphatic Monomer
| ||Sampathkumar JayaKrishnaKumar, Gunaseelaraj Rajkumar, Sengottaiyan Arul Kumar, Radhakrishnan Geethakumari |
| ||The Journal of Contemporary Dental Practice. 2019; 20(8): 940 |
|[Pubmed] | [DOI]|
||Evaluation of In Vitro Cytotoxicity of Heat-cure Denture Base Resin Processed with a Dual-reactive Cycloaliphatic Monomer
| ||Suma Karthigeyan, SreeVarun Murugesan, Balu Kandasamy, Devaki Veeramalai, Devi Natesan |
| ||The Journal of Contemporary Dental Practice. 2019; 20(11): 1279 |
|[Pubmed] | [DOI]|